Download presentation

Published byDaisy Beasley Modified over 4 years ago

1
**Prof. Juejun (JJ) Hu hujuejun@udel.edu**

MSEG 667 Nanophotonics: Materials and Devices 9: Absorption & Emission Processes Prof. Juejun (JJ) Hu

2
**Optical absorption in semiconductors**

3
**Band structure of silicon**

G : L : X : a = 5.43 Å

4
**Band structure of semiconductors near band edge**

Eg Eg k k Direct gap semiconductors: compound semiconductors Indirect gap semiconductors: group IV semiconductors

5
**Energy and crystal momentum conservation**

Energy conservation Crystal momentum conservation Thermalised electron momentum Photon momentum E k

6
**Energy and crystal momentum conservation**

Parabolic band approximation Energy conservation E EC k EV Reduced mass:

7
**Energy and crystal momentum conservation**

Energy conservation E EC k EV For a given photon energy, only a narrow band of states contribute to absorption!

8
**Electronic density of states in energy bands**

In the k-space each electronic state occupies a volume of where V is the volume of the system Dispersion relation Beware of spin degeneracy!

9
**Absorption in direct gap semiconductors**

Photon absorption rate is proportional to the joint density of states: the density of states (pairs) that can participate in the absorption process Optical transition typically does not flip the electron spin state

10
**Direct band gap energy determination**

V. Mudavakkat et al., Opt. Mater. 34, Issue 5, (2012).

11
**Absorption in indirect gap semiconductors**

Conservation laws E k Typical optical phonon energy in Si: 60 meV

12
**Absorption in indirect gap semiconductors**

Phonon-assisted absorption:

13
**Indirect band gap energy determination**

Si Appl. Opt. 27, (1988). Nanotechnology 23, (2012).

14
Amorphous solids Short range order (SRO) Lack of long range order (LRO) Properties pertaining to SRO: Energy band formation Density of states Properties pertaining to lack of LRO: Crystal momentum (not a good quantum number anymore!) Localized states (Anderson localization) Random Amorphous Unlike gases, amorphous solids are NOT completely random vs.

15
**Mobility gap in amorphous solids**

Mobility edge: a well-defined energy that separates extended states with localized states

16
**Tauc gap and Tauc plots ET = 3.3 eV Tauc gap ET definition:**

It is merely a fitting parameter and has little physical significance! ET = 3.3 eV

17
**Quasi-Fermi levels in non-equilibrium semiconductors**

Optical or electrical injection increases the density of both types of carriers In semiconductors displaced from equilibrium, separate quasi-Fermi levels, EFn and EFp must be used for electrons and holes, respectively (EFn = EFp in equilibrium) Quasi-thermal equilibrium within bands: electron relaxation time within a band is much lower than across the band gap Occupation probability in the conduction band: Occupation probability in the valence band:

18
**Absorption saturation effect**

k E Pumping Absorption saturation effect At high injection levels, the available empty states for electrons in the conduction band are depleted Equilibrium High injection level

19
**Absorption saturation effect**

k E Pumping Absorption saturation effect Equilibrium High injection level Absorption coefficient in the presence of saturation: Here EC and EV are the energies of the initial and end states

20
**Stimulated emission E k The reverse process of optical absorption**

Electron-hole recombination to emit a photon in the presence of an external electromagnetic field excitation Energy conservation Optical gain E where w is the angular frequency of the external field as well as the emitted photon k

21
**Net gain and optical amplification**

Net gain = gain – loss In practical applications, additional loss sources (scattering, FCA, etc.) need to be considered in the loss term as well Population inversion L. A. Coldren and S. W. Corzine, Diode Lasers and Photonic Integrated Circuits

22
**Stimulated and spontaneous emission**

Stimulated emission Spontaneous emission

23
**Single mode rate equation**

Consider a semiconductor with uniform carrier density n : carrier density np : photon number No carrier injection Absorption rate Stimulated emission rate Spontaneous emission rate kabs , kstim , ksp : absorption, stimulated and spontaneous emission coefficients, which are environment-independent

24
**Single mode blackbody radiator**

In thermal equilibrium Energy conservation: Hot blackbody ( ): Cool blackbody ( ): Fermi-Dirac distribution Planck distribution

25
**Single mode “hot” blackbody radiator**

In thermal equilibrium Absorption and stimulated emission dominate over spontaneous emission in a “hot” blackbody Thermal equilibrium At high temperatures, occupation probability of all states are equal

26
**Single mode “cool” blackbody radiator**

In thermal equilibrium Rereading Einstein on Radiation All the rate constants are the same specified by detailed balance Note: the rate constant ka-e is NOT a material constant as it depends on the optical mode under investigation

27
**Optical gain in semiconductors**

The absorption curve at zero injection level and the gain curve at complete inversion are symmetric with respect to the horizontal axis Their shape reflects the joint DOS in the material

28
**Optical amplification**

Gain medium Under steady-state carrier injection: Optical amplification: Optical injection Net radiative recombination Non-radiative recombination Current injection The carrier equation does NOT include optical injection at a different wavelength!

29
**Carrier density in semiconductor devices**

Solving the current continuity and the Poisson equations Current continuity Poisson equation 0 V bias 0.5 V forward bias 1-D semiconductor device simulator: SimWindows download

30
**Stimulated emission and spontaneous emission in technical applications**

LEDs Optical amplifiers Fluorescence imaging Lasers Photoluminescence spectroscopy

31
**Laser threshold Threshold Below threshold**

Spontaneous emission into multiple cavity modes dominates Gain < loss Incoherent output Above threshold Stimulated emission into usually a single mode dominates Gain ~ loss Coherent output Light intensity (L) Current (I) Even above threshold the gain is still slightly smaller than loss due to the presence of spontaneous emission b Light intensity (L) log(L) Light intensity (L) × 100 Wavelength (l) Current (I) Wavelength (l)

32
**Engineering spontaneous emission rate: Purcell effect**

Fermi’s golden rule: No photon states: suppressed spontaneous emission (SE) Photonic band gap Large photon density of states: enhanced (i.e. faster) SE rate Optical resonant cavity Enhancement factor (Purcell factor) of SE in a cavity: Initial state yi electron in CB + 0 photon Final state yf electron in VB + 1 photon In defining Purcell factor, the Q is given as min(Q_cavity, Q_emitter linewidth) n : refractive index Q: cavity Q-factor* l : wavelength V: cavity mode volume

33
**Engineering spontaneous emission rate: Purcell effect**

SE suppression SE enhancement "Investigation of spontaneous emission from quantum dots embedded in two-dimensional photonic-crystal slab," Electron. Lett. 41, (2005).

Similar presentations

© 2019 SlidePlayer.com Inc.

All rights reserved.

To make this website work, we log user data and share it with processors. To use this website, you must agree to our Privacy Policy, including cookie policy.

Ads by Google